Disorder-Order Transformation and Significant Dislocation Motion Cooperating with a Surprisingly Large Hysteretic Magnetic Transition in a Nickel-Bisdithiolene Spin System
Hai-Bao Duan; Xuan-Rong Chen; Hao Yang; Xiao-Ming Ren; Fang Xuan; Shi-Ming Zhou; Inorganic Chemistry 52 (2013) 3870–3877; doi:10.1021/ic302571p

data_4334310
_publ_section_title
;
 Disorder-Order Transformation and Significant Dislocation Motion
 Cooperating with a Surprisingly Large Hysteretic Magnetic Transition in a
 Nickel-Bisdithiolene Spin System
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              3870
_journal_page_last               3877
_journal_paper_doi               10.1021/ic302571p
_journal_volume                  52
_journal_year                    2013
_chemical_formula_sum            'C21 H11 F3 N5 Ni S4'
_chemical_formula_weight         577.30
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                71.043(5)
_cell_angle_beta                 74.970(6)
_cell_angle_gamma                77.509(5)
_cell_formula_units_Z            2
_cell_length_a                   8.2623(6)
_cell_length_b                   11.5851(6)
_cell_length_c                   13.8576(9)
_cell_measurement_temperature    190(2)
_cell_volume                     1198.86(14)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      190(2)
_diffrn_measured_fraction_theta_full 0.858
_diffrn_measured_fraction_theta_max 0.858
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0478
_diffrn_reflns_av_sigmaI/netI    0.0502
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            14915
_diffrn_reflns_theta_full        29.25
_diffrn_reflns_theta_max         29.25
_diffrn_reflns_theta_min         2.82
_exptl_absorpt_coefficient_mu    1.201
_exptl_crystal_density_diffrn    1.599
_exptl_crystal_F_000             582
_refine_diff_density_max         1.133
_refine_diff_density_min         -0.973
_refine_diff_density_rms         0.116
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.928
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     335
_refine_ls_number_reflns         5618
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.928
_refine_ls_R_factor_all          0.0785
_refine_ls_R_factor_gt           0.0552
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0962P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1378
_refine_ls_wR_factor_ref         0.1456
_reflns_number_gt                3658
_reflns_number_total             5618
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic302571p_si_002_2.cif
_cod_data_source_block           190K
_cod_original_cell_volume        1198.87(13)
_cod_database_code               4334310